- Nano Express
- Open Access
Reduced Contact Resistance Between Metal and n-Ge by Insertion of ZnO with Argon Plasma Treatment
Nanoscale Research Letters volume 13, Article number: 237 (2018)
We investigate the metal-insulator-semiconductor contacts on n-Ge utilizing a ZnO interfacial layer (IL) to overcome the Fermi-level pinning (FLP) effect at metal/Ge interface and reduce the barrier height for electrons. A small conduction band offset of 0.22 eV at the interface between ZnO and n-Ge is obtained, and the ZnO IL leads to the significant reduced contact resistance (Rc) in metal/ZnO/n-Ge compared to the control device without ZnO, due to the elimination of FLP. It is observed that the argon (Ar) plasma treatment of ZnO can further improve the Rc characteristics in Al/ZnO/n-Ge device, which is due to that Ar plasma treatment increases the concentration of oxygen vacancy Vo, acting as n-type dopants in ZnO. The ohmic contact is demonstrated in the Al/ZnO/n-Ge with a dopant concentration of 3 × 1016 cm−3 in Ge. On the heavily doped n+-Ge with a phosphor ion (P+) implantation, a specific contact resistivity of 2.86 × 10− 5 Ω cm2 is achieved in Al/ZnO/n+-Ge with Ar plasma treatment.
Germanium (Ge) has attracted much attention for the advanced metal-oxide-semiconductor field-effect transistors (MOSFETs) due to its higher carrier mobilities compared to Si [1, 2]. For the Ge p-channel MOSFETs, great progress has been made in growth of strained Ge channel [3,4,5], surface passivation [6,7,8,9], and source/drain (S/D) contacts , and the ultra-scaled Ge pFinFETs  have demonstrated the superior electrical performance to the Si devices. Ge n-channel transistors, by contrast, are still facing challenges, which produce the obstacle for the integration of Ge CMOS, including the poor interface quality, resulting in the low electron mobility, and the high S/D resistance due to the limited activation rate of n-type dopants in Ge  and the Fermi-level pinning (FLP) at metal/n-Ge interface . FLP leads to a Schottky barrier height of about 0.5 eV for electrons for most of the metals on n-Ge, producing the very large contact resistance Rc [13,14,15].
Fermi-level depinning can be done by inserting a thin interfacial layer (IL), e.g., TiO2  and ZnO , between the metals and n-Ge , due to that the thin IL can block the metal wave function into Ge to reduce the metal-induced gap states [19, 20]. ZnO has small conduction band offset (CBO) with respect to Ge, which can lead to the smaller Rc in metal/ZnO/n-Ge, compared to metal/TiO2/n-Ge with TiO2/Ge having the positive CBO . The dielectric constant of ZnO is smaller than that of TiO2, so ZnO IL can obtain a thinner depletion region between the metal and n-Ge in comparison with TiO2. In addition, it is easy to realize n-type doping in ZnO by introducing nonstoichiometric defects, such as oxygen vacancies Vo [21, 22], which gives rise to an even smaller ZnO depletion region between the metal and n-Ge. So far, in metal/ZnO/n-Ge contacts, the doping of ZnO by Vo was carried out by annealing in nitrogen atmosphere , which however, might resulted to the inter diffusion of ZnO and Ge during the annealing , and diffusion of dopant atoms in n-Ge during the annealing [24, 25], causing the degradation of current performance of the device. Since, a low-temperature process for depositing and doping ZnO needs to be developed.
In this work, we investigate the Fermi-level depinning at interface between metal and n-Ge by insertion of ALD deposited ZnO IL. The improvement effects of argon (Ar) plasma treatment of ZnO layer on contact resistance characteristics of Al/ZnO/n-Ge are studied.
Metal contacts were formed on both lightly and heavily doped n-Ge (001) wafers. The lightly doped Ge samples have a doping concentration about 3 × 1016 cm−3. To achieve the heavily doped n-Ge, a phosphor ion (P+) implant with a dose of 1 × 1015 cm−2 and an energy of 30 keV was performed on the n-Ge(001), which was followed by a rapid thermal annealing at 600 °C for 60 s. After wafer cleaning using several cycles of deionized water and diluted HCl, Ge wafers were immediately loaded into ALD (Beneq TSF-200) chamber to deposit ZnO, and then aluminum (Al) contacts were deposited by sputtering on Ge using a lift-off process. Here, three ZnO thicknesses of 1, 2, and 3 nm were utilized, which were confirmed by spectroscopic ellipsometry (SE) (J. A. Woollam M2000). During the ZnO deposition, diethyl zinc (DEZn) and deionized water (H2O) were used as the Zn and O precursors, respectively, and the substrate temperature was kept 150 °C to eliminate the formation of GeOx. The detailed ZnO deposition process using ALD was reported in our previous works in ref. [26, 27]. To further improve the conductivity of ZnO film, some ZnO on Ge samples were treated with argon (Ar) plasma. Control Al/n-Ge sample without ZnO IL was also fabricated. The Rc of Al on ZnO/Ge was extracted using the circular transmission line method (CTLM), which was formed by lift-off. The exposed ZnO was fully etched by plasma etch to ensure complete isolation between adjacent devices .
Keithley 4200 SCS was used to measure the electrical characteristics of the Al/ZnO/n-Ge contracts and CTLM structures, high-resolution transmission electron microscope (HRTEM) and X-ray photoelectron spectroscopy (XPS) were used to determine the microstructure and interface properties of the samples, and UV-VIS Spectrophotometer (LAMBDA 950, PerkinElmer) was used to determine the band gap Eg of deposited ZnO film.
Results and Discussion
Material Characterization of Al/ZnO/n-Ge
XPS valence band spectra of Ge/ZnO and transmittance spectrum of ZnO are presented in Figs. 1 and 2, respectively, which were utilized to investigate the mechanism of Fermi-level depinning effect at Al/ZnO/n-Ge interface. We conducted the XPS measurements for thick ZnO sample, ZnO/n-Ge interface sample, and pure Ge sample, to obtain the valence band offset (VBO) of ZnO/Ge, as shown in Fig. 1. The Zn 2p peak position and VBM for thick ZnO sample are 1021.9 eV and 2.59 eV, respectively. The Zn 2p and Ge 3d peak position for ZnO/Ge interface sample are 1021.7 eV and 29.1 eV, respectively. The Ge 3d peak position and VBM for pure Ge sample are 29 eV and 0.06 eV, respectively. This indicates that the VBO of ZnO/Ge is 2.33 eV .
Figure 2a shows the transmittance plot obtained from UV-VIS spectroscopy for thick ZnO sample, and the Eg of ZnO is determined to be 3.21 eV, consistent with the reported values in [28, 29]. By using the obtained Eg of ZnO and VBO above, a CBO of 0.22 eV between ZnO and Ge is determined, as shown in Fig. 2b. This indicates that Fermi-level depinning can be achieved at Al/n-Ge interface using the ZnO insertion layer, which can produce the low Rc for Al/ZnO/n-Ge contact.
Figure 3 shows the TEM image of the Al/ZnO/n-Ge structure with the thickness of ZnO of 3 nm. A uniform and conformal ZnO layer is observed between Al and n-Ge. The inset in the top right corner illustrates the HRTEM image of zoomed-in view of the Al/ZnO/n-Ge interface. The thickness of ZnO film is measured to be 3 nm, which is consistent with result obtained by SE measurement, and the ZnO film is in an amorphous form.
A thin GeOx interfacial layer is formed between Ge and ZnO, which is much smaller compared to  due to the lower deposition temperature used in this work. This is attributed to the fact that, during the deposition of ZnO, Ge reactive with O precursor, leading to the formation of GeOx IL. GeOx is also demonstrated by the XPS Ge 3d result in the inset in the top left corner.
Electrical conductivity of ZnO film can be improved by Ar plasma treatment, which causes the increasing in the concentration of oxygen vacancies Vo, acting as the donors in ZnO [32, 33]. Figure 4 depicts the XPS results of O 1s for as-deposited ZnO and the sample with Ar plasma treatment with a power of 50 W, an Ar gas flow of 60 sccm, and a duration of 45 s. The O 1s peak is deconvoluted into two peaks by using the Gaussian fitting. The peak at ~ 530 eV corresponds to lattice oxygen in ZnO [34, 35]. For the as-deposited sample, the peak at 531.7 eV corresponds to Vo (~ 531.5 eV) and chemisorbed oxygen on the surface of ZnO thin films, such as carbonyl and hydroxyl groups [35, 37]. For the sample with Ar plasma treatment, the peak is at ~ 531.5 eV, which shifts to lower binding energy, and gets much more pronounced in comparison with the as-deposited sample, indicating that more Vo are generated due to Ar plasma treatment, and chemisorbed oxygen is effectively removed. The increasing of n-type dopants in ZnO results in the thinner tunneling barrier and lower series resistance at interface, being responsible for the reduction in Rc .
We did the XPS measurements using thick ZnO sample and ZnO/Ge interface sample with and without Ar plasma treatment, as shown in Fig. 5. We found that, after Ar plasma treatment, there was a − 0.05 eV shift. This may indicate that the ZnO/Ge VBO is about 2.38 eV after Ar plasma treatment and CBO of 0.17 eV.
Electrical Performance of Al/ZnO/n-Ge Contacts
Figure 6a shows the measured current density J as a function of applied voltage V characteristics for Al contacts on lightly doped n-Ge. The Al/ZnO/n−-Ge devices have the different thicknesses of ZnO layer. The schematic of the device is shown in the inset of Fig. 6.
As predicted, the Al/n-Ge control device without ZnO shows the rectifying characteristics with the high barrier height for electrons due to the Fermi-level pinning at Al/n−-Ge . Compared with the control Al/n-Ge sample without ZnO, Al/ZnO/n-Ge devices exhibit the improved reverse J, which is due to the Fermi-level depinning induced by the reduction of metal-induced-gap-states (MIGS) at metal/Ge interface [18, 19]. This improvement is more enhanced with thicker ZnO, which is due to the fact that more MIGS are eliminated. But the forward current density for 3 nm ZnO inserted device is smaller than that of 2 nm one. This may be explained as follows. The main current density for Al/ZnO/n-Ge is tunneling current. If the ZnO is not thick enough, MIGS will not be effectively eliminated, and it still shows rectifying characteristics. But if the ZnO is too thick, the series resistance of ZnO will dominate the whole resistance, and the current gets smaller. So there is a trade-off between elimination of MIGS and increase in series resistance of ZnO, and thus there is a critical thickness for the IL . In conclusion, 2 nm is considered to be the optimal thickness for Al/ZnO/n-Ge contact.
With the Ar plasma treatment, the performance of Al/ZnO/n−-Ge device is further improved. Whatever for the reverse or forward sweeping of applied voltage V, Al/2 nm ZnO/n−-Ge device with Ar plasma treatment achieves the enhanced J compared to the device with 2 nm ZnO or 3 nm ZnO, which is due to that a large amount of Vo are generated in ZnO film during the Ar plasma treatment. The higher doping concentration in ZnO can effectively reduce the series resistance of ZnO and reduce the tunneling barrier for electrons at the interface between ZnO and Al, improving the tunneling current density.
Figure 6b shows J-V characteristics for three Al/2 nm ZnO/n−-Ge device with Ar plasma treatment. It is clear that the J for different device is nearly the same, indicating that both ALD process and Ar plasma treatment have uniform effect on the improvement of current density.
Ohmic contacts are obtained for the Al/2 nm ZnO/n−-Ge without and with different Ar plasma treatment duration of 15 s, 30 s, 45 s, and 60 s, respectively, which are shown in Fig. 7.
The raw total resistance Rtot between two contacts decreases with the decreasing of d, and the final Rtot is modified by a correction factor C, which is calculated with the equation C = (L/d)·ln(1 + d/L) , where L = 25 μm represents for the radius of inner pad, as depicted in the inset in Fig. 8a. By plotting the Rtot as a function of d in Fig. 8a, the sheet resistance Rsh of the n−-Ge can be obtained from the line slope, and then ρc is calculated from the intercept of the linear fitting line with the vertical axis. For the Al/2 nm ZnO/n−-Ge device without Ar plasma treatment, the ρc is 6.87 × 10−2 Ω cm2, but after 45 s Ar plasma treatment, there is 17.2 times reduction compared with that without Ar plasma treatment and has the contact resistivity ρc of 3.66 × 10−3 Ω cm2. We compare the values of ρc for the Al/2 nm ZnO/n−-Ge devices with different Ar plasma treatment durations in Fig. 8b. It is observed that ρc of the device decreases with the treatment time up to 30 s. However, as treatment time is larger than 30 s, ρc nearly stays the same. The reduction in ρc may be attributed to the doping of ZnO, thus to the reduction of tunneling barrier and series resistance, as has mentioned previously. But there is no observable change in sheet resistance of n−-Ge, indicating that there is no effect on the conductivity of n−-Ge with Ar plasma treatment.
CTLM structure with Al contacts on heavily doped Ge is used to investigate the contact resistance characteristic of Al/2 nm ZnO/n+-Ge. The ZnO layer underwent the Ar plasma treatment for 45 s. Figure 9a shows the measured I-V curves between the Al contacts with different d, showing the excellent ohmic performance. Figure 9b plots the Rtot as a function of d for Al/2 nm ZnO/n+-Ge CTLM, and Rsh and ρc are extracted to be 64 Ω/□ and 2.86 × 10−5 Ω cm2, respectively.
We compare the ρc of ZnO treated by Ar plasma Al/ZnO/n+-Ge devices in this work with those reported in the literature, as shown in Fig. 10. For the heavily doped n+-Ge contact sample, Al/ZnO/n+-Ge contacts shown the smaller ρc in comparison with those of Ni/GeSn [40, 41], Ni/Ge , Ti/n+-Ge in ref. , and Ti/TiO2/GeO2/Ge , carbon implanted Ni/Ge , and Ti/n+-SiGe/n-Ge . Metallic ohmic contacts such as Ni/Ge, Ni/GeSn, Ti/Ge, and carbon implanted Ni/Ge suffer from severe Fermi-level pinning, resulting in the large ρc. For Ti/TiO2/GeO2/Ge contact, a large tunneling resistance was introduced by the bilayer of 1 nm TiO2/1.5 nm GeO2 IL, degrading the contact resistivity characteristics. But the ρc in this work is larger than that in ref. . We assume that this may due to the four times larger P+ implantation dose than that in our work. Larger implantation dose will enable the heavier surface doping of n+-Ge, resulting in the thinner Schottky barrier and smaller ρc. We believe that with heavier doping of n+-Ge in Al/ZnO/n+-Ge devices, smaller ρc will result in.
The Fermi-level depinning effect induced by ZnO IL in the Al/ZnO/n-Ge structures is investigated. XPS measurement demonstrated a small CBO of 0.22 eV at ZnO/n-Ge, i.e., elimination of FLP occurs, which leads to the ohmic metal contacts on n-Ge. It is further reported that Ar plasma treatment of ZnO leads to the increasing of concentration of Vo, acting as the n-type dopants in ZnO, which improves the Rc performance in Al/ZnO/n-Ge devices. Ohmic metal contacts are obtained on n− and n+-Ge with the Ar plasma-treated ZnO IL. Based on the CTLM structures, values of ρc 3.66 × 10−3 Ω cm2 and 2.86 × 10− 5 Ω cm2 are achieved in Al/2 nm ZnO/n−-Ge and Al/2 nm ZnO/n+-Ge, respectively, with the Ar plasma treatment of ZnO at a power of 50 W for 45 s.
Atomic layer deposition
Conduction band offset
Circular transmission line method
- E g :
- GeOx :
High-resolution transmission electron microscope
Metal-oxide-semiconductor field-effect transistors
- P+ :
- R c :
- R tot :
Raw total resistance
- TiO2 :
Valence band offset
- V o :
X-ray photoelectron spectroscopy
- ρ c :
Specific contact resistivity
Shang H, Schimdt HO, Chan KK, Copel M, Otto JA, Kozlowski PM, Steen SE, Cordes SA, Wong HSP, Jones EC, Haensch WE (2002) High mobility p-channel Ge MOSFETs with a thin Ge oxynitride gate dielectric. In IEDM Tech Dig:441–443. https://doi.org/10.1109/IEDM.2002.1175873
Wu N, Zhang Q, Chan DSH, Balasubramanian N, Zhu C (2006) Gate-first Germanium nMOSFET with CVD HfO2/gate dielectric and silicon surface passivation. IEEE Electron Device Lett 27:479–481
Liu Y, Niu J, Wang H, Han G, Zhang C, Feng Q, Zhang J, Hao Y (2017) Strained germanium quantum well PMOSFETs on SOI with mobility enhancement by external uniaxial stress. Nanoscale Res Lett 12:120
Hashemi P, Chern W, Lee H, Teherani JT, Zhu Y, Gonsalvez J, Shahidi GG, Hoyt JL (2012) Ultrathin strained-Ge channel P-MOSFETs with high-K/metal gate and sub-1-nm equivalent oxide thickness. IEEE Electron Device Lett 33:943–945
Pillarisetty R, Chu-Kung B, Corcoran S, Dewey G, Kavalieros J, Kennel H, Kotlyar R, Le V, Lionberger D, Metz M, Mukherjee N, Nah J, Rachmady W, Radosavljevic M, Shah U, Taft S, Then H, Zelick N, Chau R (2010) High mobility strained germanium quantum well field effect transistor as the p-channel device option for low power (Vcc= 0.5 V) III–V CMOS architecture. In IEDM Tech Dig:150–153. https://doi.org/10.1109/IEDM.2010.5703312
Zimmerman P, Nicholas G, Jaeger BD, Kaczer B, Stesmans A, Ragnarsson LÅ, Brunco DP, Leys FE, Caymax M, Winderickx G, Opsomer K, Meuris M, Heyns MM (2006) High performance Ge pMOS devices using a Si-compatible process flow. In IEDM Tech Dig:1–4. https://doi.org/10.1109/IEDM.2006.346870
Chui CO, Kim H, Chi D, Triplett BB, McIntyre PC, Saraswat KC (2002) A sub-400 °C germanium MOSFET technology with high-ҟ dielectric and metal gate. In IEDM Tech Dig:437–440. https://doi.org/10.1109/IEDM.2002.1175872
Kuzum D, Pethe AJ, Krishnamohan T, Oshima Y, Sun Y, McVittie JP, Saraswat KC (2007) Interface-engineered Ge (100) and (111), N-and P-FETs with high mobility. In IEDM Tech Dig:723–726. https://doi.org/10.1109/IEDM.2007.4419048
Takagi S, Takenaka M (2010) III-V/Ge CMOS technologies on Si platform. In VLSI-TSA Symp Tech Dig:147–148. https://doi.org/10.1109/ISSM.1995.524390
Li R, Lee SJ, Yao HB, Chi DZ, Yu MB, Kwong DL (2006) Pt-Germanide Schottky source/drain Germanium p-MOSFET with HfO2 gate dielectric and TaN gate electrode. IEEE Electron Device Lett 27:476–478
Duriez B, Vellianitis G, van Dal MJH, Doornbos G, Oxland R, Bhuwalka KK, Holland M, Chang YS, Hsieh CH, Yin KM, See YC, Passlack M, Diaz CH (2013) Scaled p-channel Ge FinFET with optimized gate stack and record performance integrated on 300 mm Si wafers. In IEDM Tech Dig:522–525. https://doi.org/10.1109/IEDM.2013.6724666
Chui CO, Gopalakrishnan K, Griffin PB, Plummer JD, Saraswat KC (2003) Activation and diffusion studies of ion-implanted p and n dopants in germanium. Appl Phys Lett 83:3275–3277
Nishimura T, Kita K, Toriumi A (2007) Evidence for strong Fermi-level pinning due to metal-induced gap states at metal/germanium interface. Appl Phys Lett 91:123123
Gallacher K, Velha P, Paul DJ, MacLaren I, Myronov M, Leadley DR (2012) Ohmic contacts to n-type germanium with low specific contact resistivity. Appl Phys Lett 100:022113
Nishimura T, Sakata S, Nagashio K, Kita K, Toriumi A (2009) Low temperature phosphorus activation in germanium through nickel germanidation for shallow n+/p junction. Appl Phys Express 2:021202
Lin J, Roy A, Nainani A, Sun Y, Saraswat KC (2011) Increase in current density for metal contacts to n-germanium by inserting TiO2 interfacial layer to reduce Schottky barrier height. Appl Phys Lett 98:092113
Manik P, Mishra R, Kishore V, Ray P, Nainani A, Yi H, Abraham M, Ganguly U, Lodha S (2012) Fermi-level unpinning and low resistivity in contacts to n-type Ge with a thin ZnO interfacial layer. Appl Phys Lett 101:182105
Roy AM, Jason Lin JY, Saraswat KC (2010) Specific contact resistivity of tunnel barrier contacts used for Fermi level depinning. IEEE Electron Device Lett 31:1077–1079
Gupta S, Manik P, Mishra R, Nainani A, Abraham M, Lodha S (2013) Contact resistivity reduction through interfacial layer doping in metal- interfacial layer-semiconductor contacts. J Appl Phys 113:234505
Dimoulas A, Tsipas P, Sotiropoulos A, Evangelou E (2006) Fermi-level pinning and charge neutrality level in germanium. Appl Phys Lett 89:252110
Kim HK, Han SH, Seong TY, Choi WK, Seong TY (2001) Electrical and structural properties of Ti/Au ohmic contacts to nZnO. J Electrochem Soc 148:G114
Li Y, Yao R, Wang H, Wu X, Wu J, Wu X, Qin W (2017) Enhanced performance in AZO based transparent flexible TFTs due to oxygen vacancy in ZnO film with Zn-Al-O interface fabricated by atomic layer deposition. ACS Appl Mater Inter 9:11711
Biswas D, Biswas J, Ghosh S, Wood B, Lodha S (2017) Enhanced thermal stability of Ti/TiO2/n-Ge contacts through plasma nitridation of TiO2 interfacial layer. Appl Phys Lett 110:052104
Koike M, Kamata Y, Ino T, Hagishima D, Tatsumura K, Koyama M, Nishiyama A (2007) Diffusion and activation of n-type dopants in germanium. J Appl Phys 104:023523
Ajmera AC, Rozgonyi GA, Fair RB (1987) Point defect/dopant diffusion considerations following preamorphization of silicon via Si+ and Ge+ implantation. Appl Phys Lett 52:813–815
Wang T, Wu H, Chen C, Liu C (2012) Growth, optical, and electrical properties of nonpolar m-plane ZnO on p-Si substrates with Al2O3 buffer layers. Appl Phys Lett 100:011901
Wang T, Wu H, Wang Z, Chen C, Liu C (2012) Ultralow emission threshold light-emitting diode of nanocrystalline ZnO/p-GaN heterojunction. IEEE Electron Device Lett 33:1030–1032
Elam D, Nemashkalo A, Strzhemechny Y, Chen C, Ayon A, Chabanov A (2011) Studies of optical and crystal properties of ALD grown ZnO. In: Design, Test, Integration and Packaging of MEMS/MOEMS (DTIP), 2011 Symposium on, pp 185–186
Iqbal J, Jilani A, Ziaul Hassan PM, Rafique S, Jafer R, Alghamdi AA (2016) ALD grown nanostructured ZnO thin films: effect of substrate temperature on thickness and energy band gap. J King Saud University – Science 28:347–354
Jia C, Chen Y, Guo Y, Liu X, Yang S, Zhang W, Wang Z (2011) Valence band offset of InN/BaTiO3 heterojunction measured by X-ray photoelectron spectroscopy. Nanoscale Res Lett 6:316
Kim G, Kim S, Kim S, Park J, Seo Y, Cho B, Shin C, Shim J, Yu H (2016) Effective Schottky barrier height lowering of metal/n-Ge with a TiO2/GeO2 interlayer stack. ACS Appl Mater Inter 8:35419–35425
Vanheusden K, Seager CH, Warren WL, Tallant DR, Voigt JA (1996) Correlation between photoluminescence and oxygen vacancies in ZnO phosphors. Appl Phys Lett 68:403–405
Janotti A, Walle CGVD (2005) Oxygen vacancies in ZnO. Appl Phys Lett 87:122102
Kim YH, Heo JS, Kim TH, Park S, Yoon MH, Kim J (2012) Flexible metal-oxide devices made by room-temperature photochemical activation of sol–gel films. Nature 489:128–132
Zhu Q, Xie C, Li H, Yang C, Zhang S, Zeng D (2014) Selectively enhanced UV and NIR photoluminescence from a degenerate ZnO nanorod array film. J Mater Chem C 2:4566–4580
Akazawa H (2009) Argon plasma treatment of transparent conductive ZnO films. Appl Phys Express 2:081601
Kim YJ, Yang BS, Oh S, Han SJ, Lee HW, Heo J, Jeong JK, Kim HJ (2013) Photobias instability of high performance solution processed amorphous zinc tin oxide transistors. ACS Appl Mater Inter 5:3255–3261
Yu H, Schaekers M, Barla K, Horiguchi N, Collaert N, Thean A, Meyer K (2016) Contact resistivities of metal-insulator-semiconductor contacts and metal-semiconductor contacts. Appl Phys Lett 108:171602
Martens K, Rooyackers R, Firrincieli A, Vincent B, Loo R, De Jaeger B, Meuris M, Favia P, Bender H, Douhard B, Vandervorst W, Simoen E, Jurczak M, Wouters DJ, Kittl JA (2011) Contact resistivity and Fermi-level pinning in n-type Ge contacts with epitaxial Si-passivation. Appl Phys Lett 98:023702
Kim G, Kim J, Kim S, Jo J, Shin C, Park J, Saraswat KC, Yu H (2014) Specific contact resistivity reduction through Ar plasma-treated TiO2−x interfacial layer to metal/Ge contact. IEEE Electron Dev Lett 35:1076–1078
Zhang X, Zhang D, Zheng J, Liu Z, He C, Xue C, Zhang G, Li C, Cheng B, Wang Q (2014) Formation and characterization of Ni/Al ohmic contact on n+-type GeSn. Solid State Electron 114:178–181
Duan N, Luo J, Wang G, Liu J, Simoen E, Mao S, Radamson H, Wang X, Li J, Wang W, Zhao C, Ye T (2016) Reduction of NiGe/n- and p-Ge specific contact resistivity by enhanced dopant segregation in the presence of carbon during nickel germanidation. IEEE Trans Electron Devices 63:4546–4549
Raghunathan S, Krishnamohan T, Saraswat KC (2010) Novel SiGe source/drain for reduced parasitic resistance in Ge NMOS. In: In ECS Meeting, pp 71–876
Chou CP, Chang HH, Wu YH (2018) Enabling low contact resistivity on n-Ge by implantation after Ti germanide. IEEE Electron Dev Lett 39:91–94
The authors acknowledge the support from the National Key Research and Development Plan under Grant No. 2017YFB0403000, the National Natural Science Foundation of China under Grant Nos. 61534004, 61604112, and 61622405 and the founding of Jiangsu province under Grant No. BK20151250.
Availability of Data and Materials
The datasets supporting the conclusions of this article are included within the article.
YZ carried out the experiments and drafted the manuscript. GQH, YL, and JCZ supported the study and helped to revise the manuscript. HW and CL supported the deposition of ZnO. XW helped to revise manuscript. HL helped to carry out the measurements. HHZ and XC helped to deposit ZnO. YH provided constructive advice in the drafting. All the authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Zhang, Y., Han, G., Wu, H. et al. Reduced Contact Resistance Between Metal and n-Ge by Insertion of ZnO with Argon Plasma Treatment. Nanoscale Res Lett 13, 237 (2018) doi:10.1186/s11671-018-2650-y
- Fermi-level pinning
- Ohmic contact
- Argon plasma